novel linear polymers able to inhibit bacterial quorum sensing · pdf filenovel linear...
Click here to load reader
Post on 05-Mar-2018
Embed Size (px)
Novel linear polymers able to inhibit bacterial quorum sensing
Eliana Cavaleiro1,2, Ana Sofia Duarte1, Ana Cristina Esteves1, Antnio Correia1,
Michael J. Whitcombe3, Elena V. Piletska3, Sergey A. Piletsky 3, Iva Chianella2.
1 Department of Biology & CESAM, University of Aveiro, Aveiro, Portugal.
2 Centre for Biomedical Engineering, SATM, Cranfield University, Cranfield, Beds, UK
3 Department of Chemistry, University of Leicester, Leicester, UK
Bacterial phenotypes such as biofilm formation, antibiotic resistance, virulence
expression are associated with Quorum Sensing (QS). QS is a density-dependent
regulatory system of gene expression controlled by specific signal molecules, such as
N-acyl homoserine lactones (AHLs), produced and released by bacteria. This study
reports the development of linear polymers capable to attenuate QS by adsorption of
AHLs. Linear polymers were synthesized using methyl methacrylate as backbone
monomer and methacrylic acid and itaconic acid as functional monomers.
Two different QS-controlled phenotypes, Vibrio fischeri bioluminescence and
Aeromonas hydrophila biofilm formation, were evaluated to test the polymers
efficiency. Results showed that both phenotypes were significantly affected by the
polymers, with the itaconic acid-containing material more effective than the methacrylic
acid one. The polymer inhibitory effects were reverted by addition of lactones,
confirming attenuation of QS through sequestration of signal molecules. The polymers
also showed no cytotoxicity when tested using a mammalian cell line.
Quorum sensing (QS) is a refined system of communication, mediated by small
diffusible molecules called autoinducers.[1-3] Autoinducers allow the chemical
communication between bacteria in a cell-density-dependent manner.[4,5] These
molecules are produced inside the cell at low levels and diffuse outside by crossing cell
membranes. When the concentration of signal molecules in the extracellular medium
reaches a critical value, these molecules re-enter the cells, affecting their behavior.[3,5,6]
To summarize, autoinducers regulate gene expression as a function of cell population
QS is a highly specific process due to the specificity of the interactions between the
signal molecules and their receptors. N-acylhomoserine lactones (AHLs) are the most
commonly produced autoinducers of Gram-negative bacteria. The first AHL identified
as an autoinducer was N-(3-oxohexanoyl)-L-homoserine lactone (3-oxo-C6-AHL)
expressed by Vibrio fischeri. QS controls several bacterial phenotypes:
bioluminescence[10,11], conjugation , expression of several virulence factors, such as
toxins production[13,14], and development of mature antibiotic-resistant
biofilms.[15,16].The development of biofilms is an important feature for bacterial
pathogens as it provides their protection and, therefore, makes their elimination
Bacterial infections are routinely treated using antibacterial compounds that target
cellular processes such as bacterial DNA replication and repair, cell wall biosynthesis
and/or the protein synthesis. Nevertheless, bacteria can acquire resistance to these
molecules, a phenomenon increasingly reported both for the clinical and natural
environments.[20,21] Consequently, new resistant strains and even superbugs have
emerged with serious consequences for human health.
It would be desirable to be able to control the expression of virulence factors and
decrease bacterial virulence without inducing phenotypes of resistance. Since bacteria
use QS to regulate the genes, responsible for virulence and toxins production,
quenching of QS, also known as quorum quenching (QQ) may be considered as a
potential therapeutic strategy. Quorum Quenching (QQ) could be used not only to block
the formation of biofilms, but also for prevention of bacterial virulence and for the
control of any other QS-mediated mechanisms. The use of QS inhibitors offers a new
tool to fight bacterial diseases by sequestration of signal molecules at early stages of the
bacterial infections. An important advantage is that QS inhibition does not impose
selective pressure for the development of bacterial resistance, as with antibiotics.
Synthetic polymers based on methacrylates (e.g. PMMA) were successfully used to
reduce biofilm formation by Pseudomonas aeruginosa. In fact, Gottenbos and
colleagues have shown that by immobilizing positively charged methacrylates polymers
on microscope slides, the growth of Gram-negative bacteria and biofilm formation
could be prevented. Nevertheless, the effect was attributed to the positive charge of the
polymers and not to QQ.
In this work, we describe the development of biocompatible, non-cytotoxic
methacrylates polymers, which are able to sequester AHLs and interfere with QS of two
different test species: Vibrio fischeri ATCC 7744 and Aeromonas hydrophila strain
IR13.  A set of itaconic-acid/methyl methacrylate (IA-MMA) and methacrylic
acid/methyl methacrylate (MAA-MMA) copolymers were synthesized by free radical
polymerization (FRP). The study also includes the evaluation of biocompatibility and
cytotoxicity of the developed polymers by in vitro cytotoxicity tests using a mammalian
cell line (Vero cells).
2 Material and methods
Itaconic acid (IA 99 %), methacrylic acid (MAA 99 %, containing 250 ppm
monomethyl ether hydroquinone as inhibitor), methyl methacrylate (MMA 99 %,
containing 30 ppm monomethyl ether hydroquinone as inhibitor), ethylene glycol
dimethacrylate (EGDMA), acetonitrile, ethyl acetate 2-butanone, 2-methoxyethanol,
N,N-dimethylformamide (DMF), , -azoisobutyronitrile (AIBN) , N-(-
ketocapryloyl)-DL-homoserine lactone (3-oxo-C6-AHL), N-hexanoyl-DL-homoserine
lactone (C6-HSL), N-butyryl-DL-homoserine lactone (C4-HSL), Phosphate Buffered
Saline, pH 7.4 (PBS), and anti-bumping granules were purchased from Sigma
(Gillingham, UK). Nutrient Broth N 2 (NB), Luria-broth (LB) and Agar
Bacteriological (Agar N 1), were purchased from Oxoid (Basingstoke, UK).
2.2 General procedure for copolymer synthesis
A 3:1 monomer ratio was used to synthesized copolymer (or linear polymers) by free
radical polymerization: 3:1 (MMA: IA/MAA) as described in Erro! Autorreferncia
de marcador invlida.. As a polymerization solvent a mixture of 2-butanone and 2-
methoxyethanol (1:1; v:v) was used. MAA and MMA were distilled under vacuum.
Purified monomers were kept at 4 C and used without further purification. The initiator
, -azoisobutyronitrile (AIBN) was purified by fractional crystallization from ethanol
(m. p. = 104 C). Other reagents (extra-pure grade) were used without purification.
Polymerization reactions were prepared as described (Table 1). The monomers were
poured into a 250 ml three-necked round-bottom flask. The solvent mixture was added,
and a condenser and a thermometer were connected. The flask was placed on a
magnetic stirrer/heater, immersed into an oil bath and degassed with nitrogen. At 60 C,
conventional radical copolymerization started by the addition of the initiator AIBN, and
carried out for 20 h. The copolymers were precipitated, drop by drop, in ultra-pure
water, recovered by vacuum filtration (Whatman filter paper n 1) and re-dissolved in
DMF (~20-30 mL). This procedure was performed three times. The copolymers were
dried under vacuum in a desiccator at room temperature for 4 days and kept at room
temperature until use.
2.3 Linear Polymers characterization
2.3.1 Nuclear magnetic resonance (NMR) spectroscopy
The NMR spectra were obtained using a JEOL ECX-400 NMR spectrometer (Jeol,
Welwyn Garden City, UK). The NMR solvents, CDCl3 and CD3OD, were obtained
from Cambridge Isotopes Limited (UK). Twenty mg of copolymer were solubilized in
NMR solvent. Itaconic acid polymers were solubilized in methanol-d4 (CD3OD) and
methacrylic acid polymers were solubilized in chloroform-d (CDCl3). All the polymers
were analyzed by 1H NMR (400MHz). The resulting NMR spectra were analyzed with
JOEL DeltaTM data processing software.
2.3.2 Gel permeation chromatography
Gel permeation chromatography (GPC) was performed on a Polymer Labs GPC 50 Plus
system (Agilent, Stockport, UK) fitted with a differential refractive index detector.
Separations were performed on a pair of PLgel Mixed-D columns (300 7.8 mm, 5 m
bead size, (Agilent, Stockport, UK) fitted with a matching guard column (50 7.8 mm).
The mobile phase was DMF with 0.1 % LiBr (w/v) at a flow rate of 1 mL min-1.
Column calibration was achieved using poly[methyl methacrylate] standards (1.96
790 kDa, (Agile, Stockport, UK)). Samples were prepared at 15 mg mL-1 in the mobile
phase and injected (100 L) onto the column. Molecular weight and polydispersity
indices were calculated using Polymer Labs Cirrus 3.0 Software (Agilent, Stockport,
2.3.3 Binding capacity
Polymers binding capacity towards the lactones 3-oxo-C6-AHL, C4-HSL and C6-HSL